In this chapter, we introduce poly(olefin sulfone)s and review the recent progress on the photoinduced depolymerization of poly(olefin sulfone)s as well as their applications. Poly(olefin sulfone)s combined with photobase generators (PBGs) are depolymerized upon irradiation with light. A poly(olefin sulfone) is a 1:1 alternating copolymer of olefin monomer and sulfur dioxide in which the protons on the carbons adjacent to the sulfonyl groups can be readily abstracted by a base. This removal leads to a depolymerization chain reaction, resulting in incorporation of a photobase generating chromophore that can undergo a photoinduced unzipping reaction. During this reaction, the original olefin monomer and sulfur dioxide are regenerated from the primary chain of the poly(olefin sulfone). The photoinduced depolymerization of poly(olefin sulfone)s has been investigated for a wide variety of applications, including stereolithography, printable microcircuit fabrication, and removable adhesives.
- poly(olefin sulfone)s
- dismantlable adhesives
Photopolymers can change their physical and/or chemical properties through the absorption of light . Although many studies on photopolymers have been reported, a few studies show photoinduced conversion to monomers under mild conditions. If a portion of the polymer is converted completely into monomers under light irradiation, the average molecular weight decreases, and this process has potential application to sophisticated device processing, including stereolithography without solvents. Such depolymerization under mild conditions is expected to yield recyclable (and, thus, environmentally friendly or “green”) polymers. However, most of the depolymerizable polymers reported require X‐ray or electron‐beam irradiation to trigger the depolymerization process [2, 3]. Only a few reports describe use of low‐energy irradiation for the depolymerization [4, 5, 6, 7, 8, 9, 10]. The unzipping degradation of a polymer main chain containing heteroatoms by X‐ray or electron‐beam irradiation has been achieved. For a poly(1‐butene sulfone), only partial depolymerization occurs, and olefins are present in the gas produced by the irradiation [11, 12].
Degradation of a poly(olefin sulfone) doped with a photosensitizer has been investigated . The degradation of poly(1‐butene sulfone) doped with pyridine N‐oxide was induced by irradiation with 300‐nm light. In this system, however, a crosslinking reaction occurs in addition to degradation of the main chain. The number of photoinduced breaks in the main chain was 10–12. High‐efficiency depolymerization to constituent monomers was achieved for poly(olefin sulfone)s containing photobase generators using low‐energy light irradiation.
2. Poly(olefin sulfone)s
Poly(olefin sulfone)s are copolymers of olefin monomers and sulfur dioxide (Figure 1). They possess sulfonyl groups (‐SO2‐) in the main chain and are easily synthesized by radical polymerization of an olefin monomer in a liquefied sulfur dioxide . Peroxides, such as tert‐butyl hydroperoxide, benzoyl peroxide, and diethyl ether peroxides, are used as polymerization initiators. The peroxide and sulfur dioxide act as a redox initiator and generate a radical species that reacts with an olefin monomer (Figure 2). While the sulfonyl radical is fairly stable, the olefin radical is unstable. The olefin radical generated in liquefied sulfur dioxide immediately reacts with a sulfur dioxide molecule to form an alkylated sulfonyl radical. The sulfonyl radicals then react with the olefin monomers to generate a polymer chain. Note that the sulfur atom of the sulfonyl radical is positively charged; therefore, it cannot react with the sulfur atom of sulfur dioxide, which is also positively charged. In addition, the olefin monomer and sulfur dioxide form a 1:1 charge‐transfer complex in the liquefied SO2 solution. The olefin‐SO2 complex reacts like a monomer unit in the radical polymerization process. Thus, the resulting poly(olefin sulfone) is a 1:1 alternating copolymer of olefin monomers and SO2 .
2.1. Synthesis of poly(olefin sulfone)s
At ambient pressure, sulfur dioxide gas liquefies when cooled to temperatures below –10.2
3. Depolymerization of poly(olefin sulfone)s
A sulfonyl group is a strong electron‐withdrawing moiety. The electrons on the carbon atoms adjacent to the SO2 groups are attracted by SO2, and thus, the protons on those carbons are easily removed by base . When a proton on one of these carbons is removed, a chain reaction in which the main chain is depolymerized to the olefin monomer and sulfur dioxide occurs (Figure 4). Based on this process, the main chain of the poly(olefin sulfone) decomposes when mixed with bases such as piperidine, methylamine, or triethylamine. One example of base‐induced depolymerization of poly(olefin sulfone)s is reaction of poly(N, N‐diethyl 3‐butenoic amide sulfone) (DEBA) with 4,4’‐trimethylenedipiperidine (base). The 1H NMR spectrum of DEBA before addition of the base is shown in Figure 5(a). The change in the 1H NMR spectrum after addition of the base is shown in Figure 5(b). Signals of the olefin protons are easily recognized. In contrast, no change was observed in the DEBA solution without the addition of base, indicating that the decomposition of DEBA was caused by the added base. The 1H NMR spectrum of the olefin monomer (N, N‐diethyl 3‐butenoic amide) is shown in Figure 5(c). A comparison of Figure 5(b) and (c) showed that the major product in the resulting solution can be attributed to the DEBA monomer. Figure 6 shows a picture of a concentrated solution of a poly(olefin sulfone). Although the viscosity of the solution was very high, when a trace of triethylamine vapor was added to the solution, the viscosity decreased immediately.
4. Photoinduced depolymerization of poly(olefin sulfone)s
A poly(olefin sulfone) possessing a photobase generating group depolymerizes upon photoirradiation and heating (Figure 7). Poly(olefin sulfone)s that possess photobase‐generating groups were synthesized (Figures 8 and 9) . The photobase‐generating groups produce amine groups when irradiated with light. Photoinduced decomposition of the poly(olefin sulfone) was investigated using 1H NMR. A poly(olefin sulfone) film was subjected to irradiation with 254‐nm light, after which 1H NMR spectra were recorded. Figure 10(a) and (b) show the 1H NMR spectra of polymer 10 before and after irradiation, respectively, followed by heating. The progress of depolymerization was readily confirmed by the disappearance of the methylene and methine protons in the main chain (4.3–3.8 ppm), along with the appearance of signals near 5.1 and 5.8 ppm, which were assigned to protons on a vinyl group. The decomposition ratio of polymer 10 irradiated and heated under the conditions described above was estimated to be 95%. The decomposition ratio increased with the irradiation energy density (Figure 11). Conversion of the polymer to the olefin monomer (depolymerization ratio) was also estimated to be 50%. The irradiated film (polymer 10) after heating was dissolved in THF and the molecular weight measured by gel permeation chromatography (GPC) (Figure 12). The polymer completely disappeared and low‐molecular‐weight species appeared. The retention time of the lowest molecular weight species was coincident with that of the olefin monomer. The number average molecular weight decreased from 130,000 to 300.
As shown in Figure 13, a lithographic image with clear positive tone of alternating 40‐μm wide lines and gaps on a film of polymer 10 could be developed with 0.012 M aq. HCl. Irradiation with 254‐nm light triggered the generation of a base along with creation of a latent image. The visible image could be developed after heating the exposed polymer film.
5. Effect of main chain structure on depolymerization of poly(olefin sulfone)s
Photoinduced depolymerization of the polymers shown in Figure 3 mixed with a low‐molecular‐weight photo‐base generator (ANC2) was investigated . Figure 14(a) shows the change in the IR spectrum of PMPS film coated on a KBr plate without light irradiation, and Figure 14(b) shows the corresponding spectrum after light irradiation during heating (post‐exposure heat treatment). The absorption spectrum of the nonirradiated film was independent of the heating time, whereas the sulfonyl stretching bands (1311 and 1130 cm−1) decreased with the heating time after film irradiation, which indicates decomposition of the polymer main chain. The extent of decomposition increased with the irradiation energy density (Figure 14(c)), and the extent of PMPS decomposition was estimated to be 95%. Conversion of the polymer to the olefin monomer (extent of depolymerization) was estimated by 1H NMR as 92%. Therefore, the polymer was converted to monomers with very high efficiency. Figure 15(a) shows the residual ratio of the PBS sulfonyl group as a function of heating time after photoirradiation. The change in residual ratio (decomposition of the main‐chain) was slow compared to that for PMPS. In contrast, the change in the residual ratio of PMBS was as fast as that for PMPS (Figure 15(b)). The only structural difference between PBS and PMBS is the number of substituents on the main chain. Thus, the decomposition characteristics must be dependent on the structure of the main chain. Figure 16 shows the residual ratios for all polymers as a function of heating time after photoirradiation. The results show that the decomposition characteristics of the polymers can be divided into two groups: poly(olefin sulfone)s that possess only one type of proton on the main chain (branched 1‐olefins such as PMBS, PMPS, PMHS, and PMNS), and poly(olefin sulfone)s that possess two types of protons on the main chain (straight chain 1‐olefins and cycloolefins such as PBS, PPS, PHS, PcycloPS, and PcycloHS). The poly(olefin sulfone)s possessing only one type of proton on the main chain can undergo extensive decomposition, whereas the poly(olefin sulfone)s possessing two types of protons on the main chain undergo only a low extent of decomposition. The number of protons that can be abstracted appears to affect the extent of depolymerization. When many protons existing on a single main chain are abstracted, the yield of monomers was reduced, as shown in the reaction mechanism in Figure 4.
6. Poly(olefin sulfone)s possessing a photobase generator and base amplifier
Photoinduced depolymerization of poly(olefin sulfone)s possessing a base‐amplifying moiety in the side chain has been investigated using a film doped with a photobase‐generating compound . Poly(olefin sulfone)s that possess the 9‐fluorenylmethoxycarbonyl (Fmoc) group as a base‐labile N‐protecting group have been synthesized (Figure 17). The Fmoc group can undergo amine‐catalyzed thermolysis to an amino group with the evolution of carbon dioxide and dibenzofulvene [20, 21]. Therefore, the number of amino groups increased in the irradiated poly(olefin sulfone) films containing the Fmoc group and doped with PBGs during the subsequent heating step. Even though the irradiation produced few amino groups, their concentration could be amplified by the amine‐catalyzed thermal degradation of the Fmoc group. Figure 18 shows the decomposition ratio of P4 and P5 plotted as a function of irradiation energy density. The decomposition ratio of copolymer P4 was greater than that of P5. For P4, a decomposition ratio of 98% was obtained at an energy density of 900 mJ/cm2. Thus, the presence of a base‐amplifying group in the side‐chain enhanced the amount of base generated in the P4 film.
7. Poly(olefin sulfone)s composed of volatile monomers
The photoinduced depolymerization of poly(olefin sulfone)s composed of volatile olefins was investigated . The polymers were converted into volatile compounds by photoinduced depolymerization. A poly(olefin sulfone) film containing a photobase generator (ANC2) was irradiated with 254‐nm light at ambient temperature through a photomask. While very little change occurred in the film just after irradiation, the irradiated area of the film vaporized upon heating to 110
8. Application of photo‐depolymerizable poly (olefin sulfone)s to photo‐detachable adhesives
Detachable adhesives have attracted great interest due to their potential applications in reusable products and reworkable systems [22, 23, 24, 25, 26]. Adhesives used in many applications, and a variety of strong adhesives that can be employed in extreme environments have been developed . However, most high‐performance adhesives are strongly adhesive, making them difficult to remove and therefore cannot be used in recyclable materials or in reworking processes. Therefore, a need exists for glues that provide firm bonding but also can be easily detached. The strength of an adhesive bond essentially depends on surface interactions between the adhesive material and the substrate. Therefore, if the chemical structure of the adhesive material can be changed after adhesion, the adhesion strength may also change. Studies have been reported on the adhesive strength of substrates fastened using degradable polymers [23, 24, 26]. The results showed that depolymerizable polymers can act as detachable adhesives.
The adhesive strength of a poly(olefin sulfone) composed of a volatile olefin monomer and a second olefin monomer possessing a crosslinkable moiety has been evaluated . This polymer was expected to act as a detachable adhesive, as illustrated in Figure 20. When a mixture of this poly(olefin sulfone) and a crosslinking reagent was embedded between two glass plates and cured, the plates remained glued together. Subsequently, the glued plates could be separated upon irradiation with UV light and heating. For further investigation, a mixture of the poly(olefin sulfone), a cross‐linking agent, and a photobase generator were prepared, and the adhesive strengths before and after photoirradiation were examined. Figure 21 shows the chemical structures of the samples. The bond strength of the test samples was measured using a cross‐tensile test apparatus, shown in Figure 22. Figure 23(a) shows the tensile strengths obtained from plates bonded with various adhesives: cross‐linked TPAS‐11, PMPS, a commercially available epoxy adhesive (Araldite Rapid), and polypropylene. The polypropylene did not result in adhesion between the quartz plates, while the cross‐linked TPAS‐11 clearly possessed a tensile strength greater than those obtained either with the Araldite Rapid or PMPS. The superior bonding strength of the cross‐linked TPAS‐11 was thought to be due to the highly polar poly(olefin sulfone) main chain and hydrogen bonding between the carboxylic acid groups and the N‐acylurea groups at the cross‐linking sites (Figure 21). Note that PMPS‐glued plates detached upon heating to temperatures above the glass transition temperature of PMPS because it is a thermoplastic resin. In contrast, cross‐linked TPAS acted as a thermoset resin and resulted in stable adhesion. The change in the adhesive strength of the cross‐linked TPAS‐11 upon light irradiation and/or heating was also investigated. Figure 23(b) shows the tensile strength of the cross‐linked TPAS‐11 sample as prepared and after heating at 100
Photoinduced depolymerization of poly(olefin sulfone)s containing photobase generators was summarized. Since poly(olefin sulfone)s are copolymers of olefins and sulfur dioxide, the sulfur dioxide produced through the depolymerization evaporates from the system. Thus, the depolymerization reaction proceeds only in one direction, and the polymer is converted into consistent olefins. The photoinduced depolymerization of poly(olefin sulfone)s has been investigated for a wide variety of applications, including stereolithography, printable microcircuit fabrication, and detachable adhesives.